d spacing of major reflecting planes determined from TEM analysis
In the new era of communication technology there are revolutionary developments in satellite communication, global positioning systems and mobile communication systems, which has helped the developments in multilayer technologies like low temperature cofired ceramics (LTCC). The microwave electronic devices have achieved significant miniaturisation, light weight and became very cost effective using LTCC. The characteristic properties required for dielectric materials which are used in multilayers are (a) high dielectric permittivity(), (b) high quality factor (Q×f) and (c) low temperature coefficient of resonant frequency (τf). The size of the resonator is inversely related to the. Dielectric materials should posses near zero temperature coefficient of resonant frequency (τf) for thermally stable electronic devices [1-7].
Generally most of the dielectric ceramic materials are known to posses the above said properties but will sinter at temperatures above 1000 °C. Zinc niobates, ZnNb2O6 (ZN) is a low loss dielectric material with columbite structure having excellent dielectric permittivity, high quality factor and low temperature coefficient of resonant frequency. Sintering temperature of ZN is comparatively lower (~1200°C) . Hence it is widely used as dielectric resonators in microwave communication devices. In multilayer ceramic structures, the low melting electrodes such as Ag (melting point ~961°C), Cu (melting point ~1083 °C) and Au (melting point ~1064 °C) are co-fired with these ceramic materials [9,10]. In the case of Ag electrodes, processing temperature of the material must be below 950 °C.
There are several approaches to reduce the sintering temperature of the ceramics viz. (i) usage of ultra-fine particles/powders as synthesized by wet chemical methods as starting materials (ii) addition of low melting glasses to obtain a low temperature sintering composite [11-14]. Glass addition is known to be the most popular and least expensive method and hence ZN is widely used in ceramic technology.
Even though the ZN ceramics prepared by conventional ceramic route [1-6] shows excellent properties, high sintering temperature preclude its application potential in the LTCC. Usage of nano sized ZN powders (instead of micron size powders) in multi layer technology can bring down the sintering temperature to a lower value. Hence the procedure for preparing ZN ceramic powder as both micron size powders and nanosized powders and the sinterability of pure materials as well as the glass added ceramics are described in this chapter. The structural characterisation of the materials can be done using XRD and the microwave dielectric properties (in the frequency range 2-6 GHz) can be studied and compared to highlight the effect of particle size on sinterability and microwave dielectric properties of these materials.
2. Materials and methodologies
2.1. Synthesis of ZnNb2O6 using solid state synthesis technique
Single phase ZN can be prepared using oxides of Zn (ZnO 99.9+%) and pentoxide of Niobium (Nb2O5 99.9+%) as raw materials. These oxides can be weighed in stoichiometric proportion and mixed for 24h in a ball mill, using zirconia balls and distilled water as the milling medium. The slurry can be dried at 80 °C and the dried powder can be calcined at 850 °>C/4h, to get the phase pure ZN ceramics.
2.2. Preparation of ZnNb2O6 using polymer complex method
Zinc acetate [Zn(CH3COO)2 99.99%,] and niobium ethoxide [Nb(OC2H5)5, 99.95% metal basis] can be used as the starting material for preparing ZN using polymer complex method. The flow chart, in Fig. 1 shows the various steps involved in the synthesis. 3 mol equivalent of citric acid can be dissolved in 12 mol of ethylene glycol with continuous stirring for 1h to form a clear solution. 1 mol of zinc acetate can then be added and stirred for several hours at 80°C to dissolve it completely. 2 mol of Nb(OC2H5)5 can be added to this clear solution with a stirring speed of 500 rpm until it results in the formation of a thick white gel. The gel can be sonicated for 2h to obtain the uniform distribution. After sonication the polymeric precursor can be recovered by desalting with acetone. The dried polymeric precursor can be calcined at 600°C/4h to obtain the ZnNb2O6 nanopowders.
2.3. Preparation of 60ZnO-30B2O3-10SiO2 (ZBS) glass
High purity ZnO, B2O3 and SiO2 (99.9%) can be used as the raw materials for the preparation of 60ZnO-30B2O3-10SiO2 (ZBS, sintering temperature is <800 °C). The raw materials weighed accurately in the stoichiometric proportion are mixed well in distilled water medium using zirconia balls for 24 h in a ball mill. The slurry can be dried and the powder can be melted in a platinum crucible at 1000°C for 2h, and the melt can be quenched into cold distilled water and powdered. This glass powder can be used for the preparation of glass ceramic composites.
2.4. Preparation of ZN-ZBS glass composites
Appropriate amounts of ZN and ZBS glass (1,3,5,10 wt%) can be mixed using an agate mortar for 2 hours in distilled water medium and the slurry can be dried and powdered. 3wt% PVA solution can then be added to this mixture as a binder. The dried powder can be uniaxially pressed using a tungsten carbide (WC) die in the form of cylindrical discs of
diameter 14 mm and about 7 mm height at a pressure of 150 MPa. The green compact can be heat treated at different temperatures and the dimension changes are recorded. The density can be determined each time and the sintering temperature can be optimised as the temperature which gives the maximum densification.
The sintered pellets of all the compositions can powdered and the crystalline phase of the powders are identified by the XRD analysis using Cu-Kα radiation of wavelength (λ) 1.54056Ǻ for 2θ range 10-80o. The recorded patterns are compared with standard ICDD Data file with the help of Philips X’pert High Score plus software. The ZN nano particles can be characterised using transmission electron microscopy (HRTEM) FEI Technai G2 30S-TWIN high resolution electron microscope operated at 300 KV. The crystallite size, lattice parameter and the selected area diffraction patterns can be recorded using TEM. The crystallite size (d) of the nano-ZN was determined from the XRD patterns using Debye Sherrer formula [18,19],
where is the wavelength of the x-ray, is the FWHM of the maximum intense peak and is the glancing angle. The microstructure analysis of the sintered polished and thermally etched samples can be carried out using scanning electron microscope (SEM, JEOL-JSM, 5600LV, Tokyo, Japan). The bulk densities of the sintered pellets can be measured by the Archimedes method. The dielectric constant can be measured using the post resonator method of Hakki and Coleman modified by Courtney. The unloaded quality factor can be measured by a resonant copper cavity whose interiors are coated silver and the ceramic composites are placed on a low loss quartz spacer which reduces the effect of losses due to surface resistance of the cavity using a Vector Network Analyser. The temperature coefficient of resonant frequency (
The powder XRD patterns of the calcined ZnNb2O6 nanopowders are depicted in the fig 3. Fig 3(a) shows the XRD pattern of ZnNb2O6 calcined at 600°C/4h and fig 3 (b) is that of ZnNb2O6 powder sintered at 950°C/2h. The figures clearly indicate that the powder patterns are in well accordance with ICDD data card (76-1827). The average crystallite size of the nanostructured ZN calcined at 600°C/4h can be estimeted from the X-ray diffraction pattern. The fig 4 depicts the maximum intense peak obtained from XRD of ZN ceramics. Using Gaussian fit (as seen in the fig 4), the FWHM and centre of the peak can be determined. Employing Debye Sherrer formula (equation 1) the average crystallite size can be calculated as ~17 nm.
Fig 4 shows the various TEM images of ZN nanocrystallites. Fig 5 (a), (b) and (c) are the TEM images of the ZN nanocrystallites at two different regions. It can be seen that in both images the nanocrystallites have same characteristics and mostly of spherical in shape. The fig 5 (c) establishes the crystallite size at low magnification; they are well separated and have uniform size distribution. A histogram is shown in fig 5 (d), indicates the crystallite size obtained from the images both fig 5 (a) and (b). In order to obtain particle size distribution, a Gaussian function is fitted for the experimental data. The average particle size is obtained and found that it is lies between 18-20 nm. This is in good agreement with the crystallite size obtained from XRD using Debye Scherrer formula.
The high resolution TEM (HRTEM) image and the selected area diffraction pattern (SADP) of ZN nanocrystallites are shown in the fig 6 (a) and (b) respectively. Lattice plane of ZN nanoparticles are clearly visible in the HRTEM image. Inter planar spacing ‘d’ of several planes were determined using set of Fourier Transforms of lattice fringe images. TEM image analysis software (Digital Micrograph - Gatan) was used for the determination of interplanar spacing. The average d values were determined and the plane corresponding to each set of fringes are duly indexed, shown in the fig 6 (a). Interplanar spacing obtained from TEM and XRD are tabulated in table 2. Comparing the d values from the X-ray diffraction pattern, the planes corresponding to each ring was identified and indexed.
In fig 7, variation of bulk density of pellets, synthesised by solid state ceramic route and heat treated at 975°C with different wt% of ZBS is shown. From the fig 7, ZN ceramics with 5 wt% of ZBS has maximum density. Hence 5 wt% of ZBS is taken as the optimized glass addition amount for the composite. Fig 8 illustrates the variation of the bulk density of ZN and ZN-ZBS glass composites with varying sintering temperatures. From Fig. 8 it can be seen that nanostructured ZN with 5 wt% of ZBS glass has greater density at lower sintering temperatures (925oC/2h). Comparison of densification of pure (nano and micron sized) ZN ceramics shows that the densification is faster for nano powder compacts at lower temperatures, however at temperature above 1100°C for micron sized powder compacts synthesised by solid state ceramic route has higher absolute density. Since the nano powders of ZN have higher sinterability, the growth during the sintering process will be more rapid. Hence more finer intergranular porosities will be formed in the case of nano powder compacts than micron sized powder compacts. This will results in the reduction in the values of absolute densities of sintered powder compacts. Similar effects were noticed for sintered nano sized powder compacts of BZT by Manoj Raama Varma et al.  In nanostructured ZN ceramics the grain boundary area per unit volume will be more than that of the solid state synthesised ZN ceramics . This deteriorates the densification of
nano sized ZN ceramics. In the case of glass addition, low melting glasses such as ZBS enhances the sinterability of the ZN ceramic powders due to the liquid phase sintering [25,26]. The glasses start melting at lower temperatures and the molten glasses flows through the porosity between the grains and fill the porosity and the gap between the grain Boundaries . This enhances the sinterability
Fig 9 shows the SEM micrographs of the sintered ZN. Fig 9 (a) and (b) are SEM micrographs of ZN synthesised using solid state ceramic route. Large grains having average grain diameter of ~4.2 µm were observed for pure ZN. Though the sintering has taken place,
Fig. 9 (b) shows a highly densified microstructure with large amount of molten glass phases for glass-ZN composites. It is observed that by the addition of ZBS glass the grain growth decreases. In fig 9 (b) the grains have an average diameter of about 1 to 2 µm only. Fig 9 (c) shows the SEM images of the sintered nano structured ZN (obtained via chemical synthesis) which are sintered at 925 °C for 2h. The SEM micrograph exhibits highly dense grains. Average grain size obtained from the micrograph images ranging from about 1-2 µm. It reveals fine sintered grains are obtained by sintering of nano ZN powder. Fig 9 (d) shows micro structure of the nanostructured ZN ceramic powders with 5wt% of ZBS glass. Comparatively smaller grains are obtained for the glass added nano powder compacts of ZN. The densification is very high for a much lower sintering temperature viz 925oC/2hrs. Comparing all images in Fig. 9 the nanostructured ZN with 5wt% of ZBS shows very high packing with a minimum porosity at 925 °C/2h. The density and the dielectric properties viz dielectric constant, Qxf, and τf, of ZN ceramics are tabulated in table 2. Comparison of these properties of the materials synthesised by different preparation techniques reveals that the solid state synthesised shows greater values for dielectric constant and Qxf. This can be correlated with the effect of grain size. In ceramic materials the increase in the grain size deteriorates the dielectric loss. Reduction in the number of grains per unit volume, decreases of grain boundaries per unit volume and it would result in a material with a lower dielectric loss and better polarisability which improves both and Q×f [28,29]. From the SEM micrographs (Fig. 9) it can be concluded that the nanostructured ZN has more grain boundaries than solid state synthesised ZN and hence had a low and Q×f. However the glass addition to these compounds, due to liquid phase sintering the nanostructured ZN has greater densification at lower sintering temperature. The dielectric properties of micron sized ZN cermic with 5 wt% of ZBS are: density =5.48, = 21.3, τf = -66 ppm/°C and with Q×f ~38,000, sintered at 975 °C/2h. Dielectric properties of sintered nano sized ZN with 5 wt% of ZBS have density = 5.21, = 22.5, τf = -69.6 ppm/°C and with Q×f ~12,800, sintered at 925 °C/2h . Since ZnNb2O6+5wt%ZBS can be identified as one of the potential LTCC materials sintering at 925°C, co sintering studies were done with silver. ZnNb2O6+5wt%ZBS was mixed with 20wt% metallic Ag (99.99%) and sintered at 930°C/2h. SEM pictures with EDAX was recorded after sintering and found that Ag is not reacting or melting during the sintering. Hence the co sintering of ZnNb2O6+5wt%ZBS+20wt%Ag was successful as can be seen in fig.10.
|hkl Plane||d spacing from TEM (Ǻ)||d spacing from ICDD file(Ǻ)|
|Materials||Sintering temperature (oC)||Density (ρ) (g/cc)||Qxf|
|ZnNb2O6 – solid state synthesis||1200||5.32||23.3||12,800||-77.9|
|ZnNb2O6 + 5wt% ZBS||975||5.48||21.3||38,000||-66.0|
|ZnNb2O6 – polymer complex synthesis||1200||4.87||19.2||77,900||-66.4|
|ZnNb2O6 + 5wt% ZBS||925||5.21||22.5||12,800||-69.6|
Zinc Niobates ceramics were prepared in phase pure powder form using solid state ceramic technique and polymer complex method. Particle size of the ZN ceramics is determined using TEM and it is found most of the particles are in the range 18-20 nm, the particle size obtained from XRD pattern using Debye Sherrer formula is 17 nm. Effect of particle size on the sinterability and the microwave dielectric properties were studied. Micro structure shows that a high density ZN ceramics can be obtained by sintering nanopowder of ZN with 5wt% of ZBS glass at 925 oC for 2h. Optimized sintering of nano sized powder at 925 oC/2h give microwave dielectric properties of =22.5, Qxf~12,800 and τf= -69.6 ppm/oC. These composites were successfully co sintered with silver.
The influence of 26on the microwave dielectric properties of ZrTi2O6 ceramics,Parinaz RiaziKhoei, Feridoon Azough, Robert Freer, J.Am. Ceram. Soc. 89 216-223 (2006).
Characterization and Microwave Dielectric Properties of 226Ceramics, Robert C. Pullar, Jonathan D. Breeze, Neil McN. Alford, J. Am. Ceram. Soc., 88  2466-2471 (2005)
Am. Ceram. Soc., Influence of. Copper I. I. Oxide Additions. to Zinc. Niobate Microwave. Ceramics on. Sintering Temperature. Dielectric Properties. Dong-Wan Kim. Kyung Hyun. Ko Kug. Sun Hong. J. 846 1286-90 (2001).
A Nenasheva, N.F Kartenko, J. Eur. Ceram. Low sintering. ceramic materials. based on. Bi O. Zn-Nb O. compounds O. E. 2626, 1929-1932 (2006)
Low temperature sintered 26microwave dielectric ceramics doped with ZnO- 2O5additions, Jin Wang, Zhenxing Yue, Zhilun Gui, Longtu Li, J. Mater. Sci. 40, 6581-6583 (2005)
V Ovchar, A. V Kramarenko, B. Jancar, J Bezjak, D. Surnov, Inorg. Mater. 43,  227-280, (2007). Synthesis Microwave dielectric. properties of. Zn1+x Nb. O6+x A. G. Belous O.
Synthesis, characterization and microwave dielectric properties 3ATiO3 (A=Co, Mn, Ni) ceramics. P.S. Anjana and M T Sebastian. J. Am. Ceram. Soc. 89 2006 2114 2117.
Effects 2ZnCl2 addition on the ZnNb2O6 powder synthesis through molten salt method, Guo Liangzhai. Dai Jinhui, Tian Jintao, Zhu Zhibin, He Tian, Qu Xiaofei, Liu Zhongfang, Mater. Chem. and Phys. 105, 148-150 (2007).
Jantunen H. Rautioaho R. Uusimaki A. Leppavuori S. Eur J. Ceram Soc. . 20002331-36.
Sebastian M. T. Jantunen H. Int Mater. Rev 5. 200857-90.
Laren M. Ponton C. B. Mater J. Sci . 199817-22.
Renoult O. Boilot J. P. Chaput F. Papiernik R. Hubert-Pfalzgraf L. G. Lejeune M. Am J. Ceram Soc. 7512 (1992), 3337-40.
Huang C. L. Pan C. L. Mater J. Sci Lett. 2. 2002149-151.
Jantunen H. Rautioho R. Uusimäki A. Leppävuori S. Eu J. Ceram Soc. . 20002331-2336.
Synthesis of rare-earth orthoaluminates by a polymer complex method, Hirofumi Takata, Misako Iiduka, Yoshihiko Notsu, Masaaki Harada, J.Allys.Compd. 408-412, 1190 1192 2006
Direct chemical synthesis of high coercivity air-stable SmCo nanoblades, C.N.Chinnasamy, J.Y. Huang, L.H. Lewis, B. Latha, C.Vittoria, V. G. Harris, Appl. Phys. Letts. 93, 032505(2008).
Low temperature powder synthesis of 3through
Nanocrystalline materials and coatings, S.C. Tjong, Haydn Chen, Mater. Sci. Engg. 4545 (2004) 1 88.
Hynes, Robert H. Doremus, Richard W. Siegel, J. Am. Ceram. Soc. Sintering Characterization of. Nanophase Zinc. Oxide Anne. P. 858(2002) 1979-87.
Huang C. L. Weng M. H. Mater Res. Bull . 20012741-2750.
Huang C. L. Hou J. L. Pan C. L. Huang C. Y. Peng C. W. Wei C. H. Huang Y. H. Alloys J. Comp 4. 2008359-363.
Huang C. L. Shen C. H. Pan C. L. Mater Sci. Eng 145 145 2007 91 96.
Nisha and P.C. Rajath Varma, Journal of Alloys and Compounds, Sinterability studies. microwave dielectric. properties of. sol-gel synthesized. Ba Zn1 Ta2/ nanoparticles O. Manoj Raama. Varma P. 457 457 2008 422 428
Progress on grain growth dynamics in sintering of nano-powders, LIU Chunjing, Wang Xin, Jiang Yanfei, Wang Yongming, Hao Shunli, Rare Metal, Vol.25, Spec. Issue, Oct 2006 471
Singh V. K. Am J. Ceram Soc. . 1981C 133 135.
- 26. J. H. Jean, S. C. Lin, J. Mater. Res. 14 (1999) 1359-1363.
Forsterite-based ceramic-glass composites for substrate applications in microwave and millimeter wave communications, T.S.Sasikala, M.N. Suma, P. Mohanan, C. Pavithran, M. T. Sebastian, J. Alloys Comp. 461 2008 2008 555 559.
Penn, Stephen J. Webb, Lesley F. Cohen and Neil. McN. Alford, J.Am Ceram Soc. Microwave dielectric. loss of. titanium oxide. Alan Templeton. Xiaoru Wang. Stuart J. 831(1) 95-100 (2000).
Alford, Templeton, Xiaoru Wang, Meishing Xu, Michael Reece, and Kelvin Schrapel. J.Am Ceram Soc. Effect of. porosity grain size. on the. Microwave Dielectric. properties of. Sintered Alumina. Stuart J. Penn Neil. Mc N. 8071885088(1997)
Finite size effect on Sinterability and Dielectric Properties of 26Glass Composites, Mukkuttiparambil Ayyappan Sanoj, Chalappurath Pattelath Reshmi and Manoj Raama Varma, J. Am. Ceram. Soc. 92 11 2648 2653;Nov 2009